Journal of Power Sources, 26 (1989)313 -317
THE LITHIUM/TITANIUM DISULPHIDE SECONDARY BATTERY (EXTENDED ABSTRACT) K. M. ABRAHAM*, G. L. HOLLECK, and D. A. SCHWARTZ
T. NGUYEN, D. M. PASQUARIELLO
EIC Laboratories, Inc., 111 Downey Street, Norwood, MA 02062 (U.S.A.)
Introduction The availability of mixed ether electrolytes, which allow the cycling of the secondary Li electrode with high efficiency [l, 21 and the discharge of secondary Li cells at very low temperatures [ 3, 41, has prompted the fabrication of Li/TiS? cells and batteries for a variety of potential civilian and military applications [5, 61. The performance characteristics of several Li/Ti& cell and battery prototypes that we have built and tested recently are reported in this paper. Experimental The TiSz electrodes were prepared from TiS? powder synthesized using a vapor transport technique. The composition of the TiSz cathode mix used in preparing the electrodes for C-size cells was 84 wt.% Ti&, 8 wt.% C, and 8 wt.% Teflon [ 31. These electrodes had a thickness of - 0.06 cm and an area of - 200 cm’ for both sides. In order to assemble the C-size cells, the electrode package, consisting of the TiS? cathode, Celgard 2400TM separator, and L&foil anode, was spirally wound, with Li forming the outer layer of the “jelly roll”, and was inserted into ‘the C-cell can. The cells were vacuum filled with the 2_MeTHF:THF/LiAsF, (1.5 M) mixed ether electrolyte (hereafter referred to as the standard electrolyte) described previously [ 31. A few cells were also tested with other electrolyte solutions which are identified in the Results and Discussion Section. The cells were hermetically sealed. Prismatic cells having capacities ranging from 2 to 8 A h were also built and tested. The design of a 2 A h cell has been described previously . These cells formed the building blocks of a 2 A h, 24 V, rechargeable Li/TiS? battery which has the same physical size as the BB-557/U Ni-Cd and the BA-5557/U Li/SO* batteries. The larger prismatic cells had nominal capacities of 6 and 8 A h, respectively. They were fabricated in a stainless steel cell case measuring 6.12 cm X *Author to whom correspondence should be addressed. 037s7753/89/$3.50
0 Elsevier Sequoia/Printed in The Netherlands
6.04 cm X 1.65 cm. The electrode stack consisted of a number of alternate, parallel plate Li and TiS, electrodes, as in our 5 A h Li/Ti& cells, reported previously [ 51. The 6 A h and 8 A h cells were designed to yield 50 and 10, one hundred percent. depth of discharge cycles, respectively, and were intended as the building blocks of a 50 cycle or a 10 cycle, 24 V battery having the same physical size as the BB-5590/U Li/S02 or the BB-590/U Ni-Cd battery. All cells were cycled under constant current conditions using standard cycling equipment [2 - 61. Results and discussion The capacity/rate behavior of the C-cells utilizing the standard electrolyte is shown in Fig. 1. At current densities < 1.5 mA cm-‘, a capacity 2 1.6 A h (2 80% utilization) was obtained in the temperature range 20 to -20 “C. In fact, a capacity of 1.2 A h was obtained, even at -30 “C at 1.5 mA cm-*. The performance map in Fig. 1 further illustrates the excellent high-rate capability of TiSz cells. Thus, the discharge capacity at 20 “C decreases by only a small amount when the current is increased from 0.75 to 4 mA cm-*. The cycle life of the C-cells was determined by the electrolyte they contained (Table 1). The cells containing the standard electrolyte exhibited the longest cycle life, yielding > 150 cycles (Fig. 2). The Li cycling efficiency in these cells was equivalent to an F.O.M., of - 37. The Li/TiS2
Fig. 1. Performance map of Li/Ti& C-cells utilizing the standard electrolyte. hundred percent. utilization corresponds to 2.1 A h.
315 TABLE 1 Effect of electrolyte on the cycle lifea of Li/T&
Cycling parameters Electrolyteb
DischargeC current (mA)
Charge current (mA)
100% DOD cycles
Standard electrolyte THF THF:2-MeTHF: DMMd
1.6 - 2.8 1.6 - 2.8 1.6 - 2.8
320 320 320
160 160 160
160 50 35
37 19 12
aAll cycling at room temperature (20 "c). bAll electrolytes contained BMe-Furan as an additive and 1.5 M LiAsFb. CThe 320 mA corresponds to 1.5 mA cmm2. dThis electrolyte was reported in ref. 4.
2.0 CAPACITY. AH
Fig. 2. Typical cycling curves for an Li/TiSa C-cell at room temperature.
C-cell has a specific energy of 95 W h kg-’ and an energy density of 175 W h 1-l which are significantly better than the values realized in Li/Mo& (60 W h kg-’ and 135 W h 1-l) and Ni-Cd (40 W h kg-’ and 110 W h 1-l) C-cells. Comparisons of the various 24 V Li/TiS, batteries with existing Army Ni-Cd and Li/S02 batteries are presented in Tables 2 and 3. The 50 cycle Li/Ti& batteries yield about 40 times more energy than the Li/SO, primary batteries without significantly compromising the specific energy and volumetric energy density of the latter. The Li/Ti& batteries, while giving the same cumulative capacity as the Ni-Cd batteries, require fewer recharges than the latter and show significantly better charge retention on storage and low temperature discharge performance.
316 TABLE 2 Comparison of existing batteries with the 2 A h, 24 V Li/TiSz battery Chemistry
Primary 2.25 0.65 2.25 1 2.25
Rechargeable 0.5 0.1 0.4 224 81
Rechargeable 2.00 0.4 1.80 50 83
1.1 49 2.42
1.5 8 0.52
1.6 32 2.11
Rated capacity (A h) Rated discharge current (A) Capacity at 0.65 A discharge Cycle life Cumulative discharge capacity (A h) Battery weight (lb) Wt. energy density (W h lb-‘) Volumetric energy density (W h in.-3)
TABLE 3 Characteristics of larger batteries Battery designation
Li/TiSa 10 cycles
LilTiS 50 cycles
Rated capacity (Ah) Rated discharge, current (A) Capacity at 2 A discharge (A h) Cycle life Cumulative discharge capacity (A b) Battery weight (lb) Weight energy density (W h lb-‘) Volumetric energy density (W h in.-3)
Acknowledgement This work was DAAK20-84-C-0391.
References 1 K. M. Abraham, J. Power Sources, 14 (1985) 179. 2 K. M. Abraham, J. S. Foos and J. L. Goldman, J. Electrochem. 2197.
317 3 K. M. Abraham, D. M. Pasquariello and F. J. Martin, J. Electrochem. Sot., 133 (1986) 643. 4 K. M. Abraham and D. M. Pasquariello, in Proc. 32nd Power Sources Symp., Cherry Hill, NJ, 1986, The Electrochemical Society, Pennington, NJ, p. 136. 5 K. M. Abraham, J. L. Goldman and F. J. Martin, in Proc. 31st Power Sources Symp., Cherry Hill, NJ, 1984, The Electrochemical Society, Pennington, NJ, p. 98. 6 D. Schwartz, P. Hill and P. Rebe, in Proc. 32nd Power Sources Symp., Cherry Hill, NJ, 1986, The Electrochemical Society, Pennington, NJ, p. 226.